Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4868
Evaluation of Mechanical Properties of Groundnut Shell &
Date Palm Powder Reinforced Polymer Composite
B.G.S.Veerendra & U. Anil Kumar
1 PG Scholar, Department of MECH, Mallareddy Engineering College (AU), main campus, maisammaguda,
Hyderabad, Telangana, INDIA, PIN-500100 E-Mail Id: email@example.com
Assistant Professor, Department of MECH, Mallareddy Engineering College (AU), main campus, maisammaguda, Hyderabad, Telangana, INDIA, PIN-500100
E-Mail Id: firstname.lastname@example.org Abstract
The modern world can’t been imagined its development without involving the concept behind advancement in composite material. The numbers of researches are going on composite material in order to achieve desire standards. The hybrid composite have been emerged and have potential reinforcement for composites and hence gains attraction for further researches. This is due to their application for which are more benificial offer low cost, low density, tensile strength etc. The present work is on development of roofing sheet material using date palm and groundnut shell particle reinforced polyester composite. Previously, it was proven that groundnut shell particle reinforced composite is applicable to roofing sheets. This project’s main motive is to add the date palm seed powder to groundnut shell particle reinforced polyester composite to show the variation. These hybrid composites are fabricated by using hand layup method. Three samples are prepared named “A”,”B”,”C”. In which sample A is only with groundnut shell particle, sample B & C are fabricated with different proportion of groundnut and date palm seed powder. Specimens were cut from the fabricated material according to the ASTM standard for different experiments for tensile test, hardness,
and impact test. This review aims to show the improvement in properties by adding date palm seed powder to the composite material.
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4869
fastener and to hold the strands in the coveted position accordingly exchanging the outer load to support. While the other constituent is fortification, can be either engineered or characteristic filaments. The mechanical property for the most part relies on the shape and measurements of fortification. A few common filaments fortified polymer composites are brought into the focused market for the request of expanding condition security. Grids which utilized are either thermoset or thermoplastic. Ordinarily utilized saps are thermoset framework Polyester, Epoxy and phenolic. while polypropylenes, polyethylene and elastomers goes under thermoplastic network.
Epoxy resins are nothing but polyether resins which contains more than one epoxy group capable of being converted into the thermoset form. Because of their following characteristics of epoxy or polyester resin systems are used for preparing composite components.
Botanically, groundnut is known as Arachishypogeae belongs to the family Leguminosae. Fourth largest oilseed production in the world is from groundnut. Groundnut is the second largest producer in India after china. The complete seed of groundnut is known as pod and outer most layer of groundnut is called shell. The lignin proportion of groundnut shell fiber is much greater than that of baggase, rice, banana, jute, hemp, husk, kenaf and sisal fibers. The content of hemicelluloses of the fiber is 18.7%, lignin 30.2%, cellulose 35.7% and ash 5.9% content. In these, lignin is called as cementing agent, which binds fiber of individual cells together. The hemi celluloses is preferred for moisture absorption.
For many years, the date palm phoenix dactylifera playing an important role in day-to-day life for the people. Today worldwide utilization, production and industrialization of dates are all continuously increasing, has rich content of nutrients for which it earned great importance. Date pits are considered as waste which represents average of 10% of date fruits. Mechanical properties like corrosion resistance, strength, wear resistance are acquires to improve extensively by adding hard fillers. Few aspires of engineering polymers are ease of fabrication, density, corrosion resistance. Upon particle reinforced polymer matrix development cost reduction and stiffness improvement qualities are scope for commercial requirements]. The useful filler particle to improve mechanical, thermal and electrical properties is silica which is proven. Increase in fatigue and flexural strength increment in surface area of particle reinforced noticed by Nakamura et al.
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4870
water absorptivity esteem ,with the most astounding effect esteem.
S.Muthukumar, K.Lingadurai(2014): Paper investigation is on developing of PMC using coconut shell powder and groundnut shell powder in different volume and found its tensile strength, impact strength and flexural property with engineering properties. The resultant composites are more environmental friendly and used in automobile, railway coach, military applications.
G.C. Onuegbu et al(2013): Explored the mechanical properties of polypropylene composites with ground nut husk powder at various molecule sizes and found that the nearness of ground nut husk enhanced the rigidity, modulus, flexural quality and effect quality of the composites.
Investigation was in the utilization of Groundnut shell as fine total fortification substitution. The appropriateness of groundnut shell powder as a constituent material in concrete was done investigaion by supplanting extents by their volume of fine total with groundnut shells. Physical properties of groundnut shells, concrete and totals were resolved. Cement of size measuring 150x150x150mm were thrown. Increment in level of groundnut shells in the threw block prompted a comparing diminishment in densities and compressive quality esteems. At a substitution of 25% esteem or more, of fine totals with groundnut shells; lightweight cement were delivered which could be utilized where low anxiety is required. MATERIALSANDMETHODS
In this chapter we deal with the materials that are used in the study of the materials are processed and its methods.
The materials that are used in the present concern of Studies are:
1. Matrix material
Composite material is a multi-stage framework comprised of grid material and fortifying material. Lattice material is a nonstop stage, and it incorporates metal network composite materials, inorganic non-metallic grid composite materials and polymer framework composites by the diverse network materials.
Matrix material serves several functions, the important ones being:
-It binds the fibers together. -It supports the overall structure.
-Protects the composites from the incursion of external agents such as chemicals, humidity, etc. -Transfers stresses and loads within the composite structure.
- Protects the fibers from damage due to handling. Table 3.1 matrix material temperature comparison
Performance of polymers is highly sensitive to several environmental variables. For instance, while mechanical properties of metals are temperature sensitive only in proximity of melt temperature, polymers’ mechanical properties are highly sensitive to heat.
a) Polyester resin
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4871
Figure: 3.1 polyester resin
Across-linked unsaturated polyester resin of a linear unsaturated polyester with the following structure b) MEKP Hardener
MEKP is a Liquid Hardener. MEKP is made out of methyl ethyl ketone peroxide, an impetus, added to polyester and vinyl saps. At the point when MEKP is blended with the tar, the subsequent substance response makes warm develop and cure or solidify the gum. MEKP Catalyst is regularly added to polyester pitch at a proportion of in the vicinity of 1 and 3%, as per the pot-life and cure speed required and the encompassing temperature. Continuously take after the rules that go with your particular tar framework
Figure: 3.2MEKPHardener c) Cobalt octoate Accelerator
A quickening agent is added to the catalyzed sap to empower the response to continue at workshop temperature and additionally at a more prominent rate. Since quickening agents have little effect on the sap without an impetus they are
now and again added to the pitch by the polyester maker to make a 'pre-quickened' gum. Cobalt is a typical quickening agent. Cure is exothermic: as the parts crosslink, they discharge warm.
Figure: 3.3 cobalt octoate 2) Filler Materials
a) Groundnut shell powder
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4872
figure: 3.4 groundnut shell powder b) Dates seed powder
Date seeds, which constitute 6-15%of the total weight of the ripe date. Date seed containsonly10% of moisture and remaining contains90% contains dry matter which fixed ash content is about 5.67%and major constituents are magnesium and calcium and minor traces of phosphorous, iron. The date seed of enough quantity were collected and dried it in sunlight. The dried date seed were washed thoroughly with water to take away the sand particles and other impurities. Then the shells dried and hammered to reduced to its size to smaller and grinded in a machine to make sure the particles were sieved to less than 1mm.
Figure: 3.5 dates seed powder Fabrication:
Mixtures with polyester resin, accelerator and corresponding catalyst as recommended are prepared to fabricate the composite. Groundnut shell and date seed powder with an average particle
size of less than 1mm are filled in polyester resin matrix to prepare the composites.
Table 4.1 Preparation of samples through hand layup process
SAMPLES Composition Volume(%) sample
Polyester resin + groundnut shell powder
Polyester resin + groundnut shell powder + dates seed powder
Polyester resin + groundnut shell powder + dates seed powder
Preceding assembling, numerous materials, outline, and creation choices are made to guarantee item unwavering quality and legitimate execution. To approve these choices, an assortment of testing strategies are utilized. The techniques are gathered into two noteworthy classes:
• Mechanical Testing
• Non-Destructive Testing (NDT)
Mechanical testing, which is also known as destructive testing, is accomplished by forcing a part to fail by the application of various load factors. In contrast, non-destructive testing does not affect the
0 20 40 60 80 100
sample 1 sample 2 sample 3
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4873
part’s future usefulness and leaves the part and its component materials in tact.
This test is carried out with accordance of IS 1608:2005. This testing process involves the test specimen to be placed in a testing machine and applies tension to it till it get fractured. The tensile force recorded as function of increase in the gauge length. A point load was applied along the center of the span of the corrugation. The maximum load at the point was noted, which gives the splitting load for the corrugated specimen.
Figure: 5.1 Test piece B)HardnessTest
Hardness is a normal for a material, not a basic physical property. It is characterized as the protection from space, and it is dictated by measuring the perpetual profundity of the space. This test is completed with understanding of ASTM D 2240. C) Impact Test
Amid the testing procedure, the example must be stacked in the testing machine and permits the pendulum until the point when it cracks or breaks. Utilizing the effect test, the vitality expected to break the material can be measured effectively and can be utilized to gauge the durability of the material and the yield quality. Impact tests measure resistance to shock loading or impact by determining the amount of energy
absorbed by the test specimen. There are two basic types of impact tests:
• Pendulum • Drop Weight
Results Tensile Test
The results obtained for the tensile test is shown below
S : samples b : Width (mm) t : thickness (mm) A : Area (mm²) L : Load (KN)
TS : Tensile strength (N/mm²) Table 6.1 Tensile test results
s b t A L TS
1 12.4 9
2 15.3 4
18.10 5 3 12.7
The results obtained for the tensile test on heating specimen up to 200°C
Table 6.2 Tensile test results on heating specimen
s b t A L TS
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4874
7 4 3
2 12.7 12. 5
158.75 1.2 4
15.62 2 3 12.2
Hardness Test (shore D)
The results obtained for the hardness test is shown below
Table 6.3 Results for hardness test
Sample 1 78
Sample 2 80
Sample 3 85
Percentage elongation: At room temperature
At 200°C temperature
Tensile strength: At room temperature
At 200°C temperature
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4875
Mechanical testing reports Impact test report
Hardness test report
The aim of the project is to develop the groundnut shell reinforced polyester composite by adding date seed powder as reinforcement.
Three different grades of sample roofing sheets were produced, the samples differ from one another by varying the reinforcement particles with same proportion of polyester resin during production.
Sample C had the highest tensile strength of 18.188N/mm² followed by sample B and A of 18.105 N/mm² and 15.711 N/mm² respectively
Likewise hardness of sample C had highest followed by sample B and A respectively.
It was found that variation shown in impact test is far less, as the proportion of shell powders is less in quantity .
Sample C has the best possible proportion than sample B and A to be taken into consideration for the production of commercial use. Sample “C” was adopted in this work because of its excellence performance properties. The results revealed that addition of date seed powdered particles with groundnut shell particles can be used as reinforcement for polymer matrix for the production sheets.
 Jacob Olaitan AKINDAPO1, Umar Alhaji
BINNI1, Olawale Monsur SANUSI2
 Had done project on groundnut shell powdered
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4876
particles as reinforcement implies more strength, especially hardness.
 R.N. Rothon, Mineral fillers in thermoplastics: filler manufacture, J. Adhesion, 64 (1997) 87–109.
 L.E. Nielsen and R.F. Landel, Mechanical
properties of polymers and composites. seconded. Marcel Deckker, New York, 1994, pp.377–459.
 I.Yamamoto, T. Higashihara and T.
Kobayashi, Effect of silica-particle characteristics on impact/usual fatigue properties and evaluation of mechanical characteristics of silica- particle epoxy resins, Int. J. JSME, 46 (2) (2003) 145– 153.
 G.C. Onuegbu, S.C. Nwanonenyi,
M.U.Obidiegwu "The Effect of Pulverised Ground Nut Husk on Some Mechanical Properties of Polypropylene Composites", International Journal of Engineering Science Invention, Vol.2(6), pp.79‐ 83, 2013.
 Vasanta V Cholachagudda , Udayakumar.P.A ,
Ramalingaiah "Mechanical characterisation of coir and rice husk reinforced hybrid polymer composite", International Journal of Innovative Research in Science, Engineering and Technology ,Vol. 2(8),2013.
 G. U. Raju, V. N. Gaitonde, S. Kumarappa, "Experimental Study on Optimization of Thermal Properties of Groundnut Shell Particle Reinforced Polymer Composites", International Journal of Emerging Sciences, Vol .2(3), pp 433‐ 454, 2012.
 S.Muthukumar, K.Lingadurai "Investigating the mechanical behaviour of coconut shell and groundnut shell reinforced polymer composite", Global Journal Of Engineering Science And Researches, Vol.1(3) pp 2348 – 8034, 2014.
 P. Procter, J. Solc, Improved thermal
conductivity in microelectronic encapsulants. IEEE Trans on Hybrids ManufTechnol, 14(4) (1991) 708–13.
 Y. Nagai, G.C. Lai, Thermal conductivity of epoxy resin filled with particulate aluminum nitride powder, J. Ceram SocJpn, 105(3) (1997) 197–200.
 N.M. Sofian, M. Rusu, R. Neagu and E. Neagu,
Metal Powder-filled Polyethylene composites, V.thermal
properties, J.thermoplastic composite materials
 Y.P. Mamunya, V.V. Davydenko, P. Pissis and E.V. Lebedev, Electrical and Thermal Conductivity of Polymers Filled with Metal Powders, J. European Polymer,38(9)(2002)1887-1897
 Patnaik Amar, Md. Abdulla, SatapathyAlok , B. Sandhyarani and K. S. Bhabani, A study on a possible correlation between thermal conductivity and wear resistance of particulate filled polymer composites, J. Materials and Design ,(In press) (2009).
 Tsao T.N.G., Thermal Conductivity of Two
Phase Materials, J. Industrial and Engineering Chemistry, 53(5) (1961) 395–397.
 Cheng S.C. and Vachon R.I., The Prediction of the Thermal Conductivity of Two and Three Phase Solid Heterogeneous Mixtures,B.Tech Thesis 2014 Mechanical Engineering Department, N.I.T. Rourkela Page 31 Int. J. of Heat Mass Transfer, 12(3) (1969)249–264.
 Oksman K., Mathew A. P., Långström R.,